Save this PDF as:

Size: px
Start display at page:

## Transcription

1 Problem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength - high conductivity electrical leads to integrated circuits (pure gold as you may know is rather soft). The high conductivity requirement dictates that the Au matrix in which the precipitates are formed should be as pure Au as possible. The phase diagram of 4 different alloy systems, Au-Ag, Au-Ni, Au-Si and Au-Co, are given below. a) Which of these systems could you heat treat to produce precipitation from a high wt% Au solid solution? Give reasons why you rule out any of these systems. A: I would choose Au-Ni, or Au-Co where there can be significant amounts of the second component dissolved in a Au-rich solid solution but where that solubility decreases with decreasing T. Au-Si won t work because almost no Si can be dissolved in the Au solid solution. Au-Ag doesn t work because Au and Ag are completely soluble in the solid state just as they are in the liquid. There is thus no way to precipitate any particle from the solid solution. b) If there is more than one system in a) that can be heat treated to produce precipitates, which one would you pick to satisfy the high electrical conductivity criterion and why? A: I would Au-Co over Au-Ni, because from the phase diagram the solubility of Co in (Au) is less than the solubility of Ni in (Au) at any aging temperature. Thus after precipitation the (Au) matrix will be purer Au in the case of Au-Co. c) What would be the overall composition of the alloy you would try first? What would be the approximate composition of the precipitate you would expect to produce? A: Au-6 to7wt%co since a maximum of 8% can be dissolved at ºC, the precipitate would be ~100%Co (eco phase) at any temperature below 400 ºC. d) Describe the steps in the process you would use to produce precipitate particles. Give all pertinent information necessary for someone to duplicate your treatment and tell why each step is necessary. A: The first step is to solutionize by holding the Au-Co at about 990 ºC. The next step is to quench the alloy, that is, rapid cooling by putting it in water. Then the alloy is aged by raising the temperature so that the Co can diffuse. First forming a high number density of nuclei during the heating and then aging at a fixed temperature to allow the precipitates to grow and then coarsen until they are of optimum size and spacing (just large enough to resist cutting by dislocations but having the smallest spacing possible for that size. The exact time and temperature of the aging cannot be determined without a TTT curve for the specific composition.

2

3

4

5

6 HW#7 Problem 2 a) An alloy knife blade of 14 at.% Be in Ni is held at 700 o C for several months. i) What is (are) the phase (s) present and its (their) composition? i) 14 at % Be in Ni = 86 at % 700 o C and 86 at% Ni in Ni!β and Ni phases are present Compositions: Drawing a tie line at 700 o C and 86 at% Ni between the β and Ni phases, we see that the β phase contains 51 % Ni and the Ni phase contains 95% Ni. ii) If there is more than one phase give the wt% of each phase present (at 700 o C) in the microstructure. ii) To calculate wt%, we can simply use the 2 nd phase diagram for Problem 2, which is as a function of wt% Ni. Drawing a tie line at 86 at % Ni (this is equivalent to 97 wt % Ni-see diagrams) and using the lever rule we obtain: wt % β = ( )/ ( ) = 13.0% wt % Ni = (97-87)/( ) = 87%

7 51 % 95 % 86 at% 97 wt b) Your boss suggests a precipitation hardening heat treatment to produce maximum hardness as follows. i) Heat rapidly from 700 o C to 1170 o C, hold for 1 hr. ii) Quench in ice water iii) Reheat to 1050 o C to age precipitation harden for 5 hours.

8 Do you agree? If not, write a diplomatic < 1 page memo discussing what is wrong with her suggestion and outlining what changes you would make to the heat treatment procedure and why. b) The precipitation hardening procedure that I would recommend would be to 1) heat rapidly from 700 o C to between o C. You want to heat above the solvus line at T~ 1080 o C but below the eutectic temperature of T=1150 o C. Above 1150 o C melting from the nonequilibrium microconstituent could occur. Therefore, we want to heat at a temperature between o C. At this point, the alloy would only contain Ni in its structure, which we call a solid solution. 2) I would then quench or cool rapidly which would prevent the atoms from diffusing to potential nucleation sites and therefore the β phase would not form. At this point the structure still only contains Ni, which is now a supersaturated solid solution containing excess Ni. This is not an equilibrium structure. 3) The last step would be to age or precipitate harden at an appropriate temperature and time to form finely dispersed β precipitates. The yield strength of the alloy is dependent on the aging temperature and time. From lecture, we saw that a copper alloy exhibited a maximum yield stress after aging for ~ 1-2 hours. For higher aging temperatures, shorter times are needed because diffusion is rapid and the precipitates form quicker. Thus, to age harden at 1050 o C for 5 hours as suggested in the problem is too excessive. I would recommend an aging time between 200 and 460 o C for ~1-2 hours.

9 Problem Set 7 3.) The compositions and isothermal transformation diagrams for two steels are given below. Steel A wt.% C, 0.29 wt.% Mn, balance Fe Steel B wt.% C, 0.56 wt.% Mn, 3.53 wt.% Ni, 0.74 wt.% Mo, balance Fe The isothermal transformation diagrams for the two steels are shown below. You may also want to consult the phase diagram for the Fe-C alloy system, which you can find in the lecture viewgraphs for lecture 15 or 16. (A word to the wise: I expect you to memorize the part of this phase diagram that is important for the heat treatment of steels and I will feel free to give you future problems on homeworks, quizzes and the final exam that require you to supply this information.)

10 a) How would you measure the hardenability of each steel? b) Which steel will have the highest hardenability? Why? c) Thin razor blades of each steel are heated to 950 C and then quenched in ice water. Describe the microstructure of each blade? Which blade will have the highest hardness? Why? d) How would you produce spheroidite (a morphology that consists of spheres of Fe 3 C in? - Fe) starting from the samples in c)? Which sample would have the higher percentage of cementite, if that phase forms?

11 A: a) Hardenability is the ability of an alloy to be hardened by the formation of martensite as a result of a given heat treatment. To test this, one should use the Jominy end quench test, which involves cooling a bar of steel from one end, and then measuring the hardness as a function of distance from the cooled end. b) Steel B should have the highest hardenability because the austenite to pearlite transformation is pushed back relative to Steel A, so that transformation can be more easily avoided. The result is that more martensite will be formed further from the quenched end in Steel B. c) Quenching in ice water produces very rapid quenching rates, fast enough ot avoid the austenite to F+C as it goes through this area of the TTT diagram. Thus the austenite of both steels will transform to martensite with a lenticular, plate-like morphology but the martensite of steel A will have a higher C content and will thus have a higher yield stress and hardness due to the strong interaction between the elastic dipoles formed by the C interstitial atoms in martensite and dislocations. Remember what makes martensite hard is carbon but whether martensite will form at all depends on the hardenability of the steel, which may be changed by changing the concentration of certain substitutional alloying elements. d) Spheroidite can be produced by heating to just below the eutectoid temperature (~ 600 C) and holding for a long time (~20 hrs). This allows the carbon to diffuse and precipitate from the martensite phase as the Fe 3 C or cementite phase. Once all the C is gone from the martensite, it is bcc Fe or ferrite. The Fe 3 C phase forms as sphere-like particles to reduce the high energy boundary area between phases. In this case, Steel A would have the higher percentage of cementite due to its higher carbon content.

12 Yes, martensite will form. The martensite will be found near the interface between the weld and the metal plate along the length of the weld where the metal plate has melted. The martensite that forms comes from the 0.8 wt% C metal plate of moderate harden-ability. The medal welding rod, of low hardenability, that is melted into the groove to form the weld will not form martensite The cooling rate at this interface should be greater than the 200 o C/s needed to miss the C- shape of the Isothermal Transformation Diagram to the left and reach the martensite formation temprature. Thus the melted portion of the eutectoid steel along the weld bead will be quenched into the martensite phase. The welding rod has a low carbon content (it has low hardenability). It is safe to assume that the cooling rate to room temperature will not be fast enough to quench the steel in the martensite phase. The cooling rate needed to quench pure steel into the martensite phase is about 10 3o C/s. The region further away from the weld is not heated to a temperature above the eutectoid temperature and does not form austenite. Because no austenite forms, martensite can not form here.

13 Question 4 Two batches of aluminum (99% pure) wire are produced from inch diameter cylindrical rod stock by drawing through a die at 25 o C. The rod stock has been annealed prior to drawing. Batch A was uniformly drawn to a diameter of inch whereas batch B was uniformly drawn to a diameter of inch. The yield stress σ y of batch A wire was 69 MPa, and σ y of batch B wire was 138 MPa, whereas σ y of the original rod stock was 55 MPa. The magnitude of the dislocation Burgers vector in Al is 0.29 nm and the shear modulus equals 28 GPa. a) (i) Estimate the dislocation density in the wire from each batch if the initial dislocation density of the rod stock was /m 3. Ans: ρ A = 7.4*10 13 m -3 and ρ B = 2.61*10 15 m -3 The initial dislocation density is ρ = /m 3. Now, we use the equation: σ o = σ y,i - α G b (ρ) 1/2 where we assume α to be 0.2. Using values provided, we calculate for σ o. σ o ~ 55 MPa Notice that the annealing has little effect on the yield strength of the material. We then solve for the new dislocation density for the two drawn samples: ρ A = [(σ t,a - σ o ) / (α G b)] 2 = [(69-55)/(0.2*(28E3)*(0.29E-9)] 2 = 7.4*10 13 m -3 5

14 ρ B = [(σ t,b - σ o ) / (α G b)] 2 = [(138-55)/(0.2*(28E3)*(0.29E-9)] 2 = 2.6*10 15 m -3 (ii) What would the dislocation arrangement in batch B wire look like under the electron microscope? (You may draw a picture). Comment on any significant features of this structure. Ans: see micrograph from lecture (slide 3, lecture 18) Because the dislocation density of sample B is extremely high, we expect the dislocations to arrange in a cell-like structure as shown in the micrograph above. b) Specimens from batches A and B are heated to 250 o C along with a piece of the original rod stock. The recrystallization temperature of Al is ~250 o C and the critical true strain is (i) Plot the changes you would observe in σ y (measure at 25 o C) as a function of time held at 250 o C for each of the specimens. Ans: True strain = ln (A o /A) = ln(d o 2 /d 2 ) = 2ln(d o /d) where A is the cross-sectional area of the rod and d is its diameter. The true strains of the samples are: ε original = 0 ε A = 2 ln(0.1/0.08) ~ 0.45 ε B = 2 ln(0.1/0.01) ~ 4.6 The original sample, having been annealed, is beneath the critical true strain. Therefore no recrystallization takes place. Samples A and B are strained above the critical value and we would expect recrystallization to take place. This means that in both cases, the dislocation density decreases as a function of time at 250 o C as new, dislocation-free grains nucleate and grow (The actual rate of recrystallization for the more highly strained sample B is faster than that of sample A so the yield stress of sample B should decrease before sample A the reverse of what is shown in the figure). When the microstructure of the two samples begin to look essentially like that of the original, we obtain our original yield stress (see plot).

15 yield stress, σ y original sample B sample A Annealing time

16 (ii) After holding at 250 C for 10 hours will there be any differences in the grain size of the two specimens of batch A and B? If you claim that differences will exist, explain why. Ans: Yes. Since regions of high dislocation density are starting points for the recrystallization process, we would expect the sample with higher ρ to initiate more new grains. Therefore sample B will have smaller grain size than sample A, which recrystallized with fewer nucleation centers. Fewer nucleation centers would result in larger grain size, as would be the case for sample A.

17

18

### Chapter Outline: Phase Transformations in Metals

Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations

### Iron-Carbon Phase Diagram (a review) see Callister Chapter 9

Iron-Carbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,

### = 62 wt% Ni-38 wt% Cu.

9-2 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,

### Introduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010

Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal

### The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R

3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated

### Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular

Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation

### 9.11 Upon heating a lead-tin alloy of composition 30 wt% Sn-70 wt% Pb from 150 C and utilizing Figure

9-13 9.8: 9.11 Upon heating a lead-tin alloy of composition 30 wt% Sn-70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition

### Introduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1

Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic

### Heat Treatment of Steels : Spheroidize annealing. Heat Treatment of Steels : Normalizing

Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should

### Module 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV

Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &

### Experiment: Heat Treatment - Quenching & Tempering

Experiment: Heat Treatment - Quenching & Tempering Objectives 1) To investigate the conventional heat treatment procedures, such as quenching and annealing, used to alter the properties of steels. SAE

### Phase Transformations in Metals and Alloys

Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press

### MSE 528 - PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY

MSE 528 - PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of Al-Zn-Mg-Cu high strength alloy on isothermal

### Heat Treatment of Steel

Heat Treatment of Steel Steels can be heat treated to produce a great variety of microstructures and properties. Generally, heat treatment uses phase transformation during heating and cooling to change

### Alloys & Their Phase Diagrams

Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Consider the Earth

### Lecture 18 Strain Hardening And Recrystallization

-138- Lecture 18 Strain Hardening And Recrystallization Strain Hardening We have previously seen that the flow stress (the stress necessary to produce a certain plastic strain rate) increases with increasing

### Solution for Homework #1

Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen

### Development of High-Strength Steel Wire with Superior Weldability

INDUSTRIAL MATERIALS Development of High-Strength Steel Wire with Superior Weldability Hiromu IzumIda*, Kenichi SHImIzu, Shinei TaKamura, Yasuhiro SHImoda, osamu momozawa and Teruyuki murai High-carbon

### The mechanical properties of metal affected by heat treatment are:

Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.

### LABORATORY EXPERIMENTS TESTING OF MATERIALS

LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective

### CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS

7-1 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length

### CHAPTER 9 Part 1. = 5 wt% Sn-95 wt% Pb C β. = 98 wt% Sn-2 wt% Pb. = 77 wt% Ag-23 wt% Cu. = 51 wt% Zn-49 wt% Cu C γ. = 58 wt% Zn-42 wt% Cu

CHAPTER 9 Part 1 9.5 This problem asks that we cite the phase or phases present for several alloys at specified temperatures. (a) For an alloy composed of 15 wt% Sn-85 wt% Pb and at 100 C, from Figure

### Materials Issues in Fatigue and Fracture

Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view

### Strengthening. Mechanisms of strengthening in single-phase metals: grain-size reduction solid-solution alloying strain hardening

Strengthening The ability of a metal to deform depends on the ability of dislocations to move Restricting dislocation motion makes the material stronger Mechanisms of strengthening in single-phase metals:

### Tensile Testing. Objectives

Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able

### MARTENSITIC STAINLESS STEEL RWL-34

MARTENSITIC STAINLESS STEEL RWL-34 RWL 34 is a Rapid Solidified Powder (RSP) Martensitic Stainless Steel, which is variation of the 420 martensitic stainless steel family with minimum 13 percent chromium

### ALLOY 800 / 800H / 800AT DATA SHEET

ALLOY 800 / 800H / 800AT DATA SHEET UNS N08800 / UNS N08801 / UNS N08811 GENERAL PROPERTIES ////////////////////////////////////////////////////// //// 800 (UNS N08800), 800H (UNS N08810) and 800AT (UNS

### BINARY SYSTEMS. Definition of Composition: Atomic (molar) fraction. Atomic percent. Mass fraction. Mass percent (weight percent)

BINARY SYSTEMS Definition of Composition: Atomic (molar) fraction Atomic percent Mass fraction Mass percent (weight percent) na =, x i n = A i i i Weight percent mainly in industry! x at % A = x 100 A

### HEAT TREATMENT OF STEEL

HEAT TREATMENT OF STEEL Heat Treatment of Steel Most heat treating operations begin with heating the alloy into the austenitic phase field to dissolve the carbide in the iron. Steel heat treating practice

### Heat Treating of Nonferrous Alloys

Metallogr. Microstruct. Anal. (2013) 2:190 195 DOI 10.1007/s13632-013-0074-8 TUTORIAL Heat Treating of Nonferrous Alloys Howard E. Boyer Ó American Society for Metals 1984 The reader should understand

### Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139

Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 5 Heat Treatment of Plain Carbon and Low

### Development of API X80 Grade Electric Resistance Welding Line Pipe with Excellent Low Temperature Toughness

JFE TECHNICAL REPORT No. 12 (Oct. 2008) Development of API X80 Grade Electric Resistance Welding Line Pipe with Excellent Low Temperature Toughness NAKATA Hiroshi *1 KAMI Chikara *2 MATHUO Nobuyuki *3

### API X80 Grade Electric Resistance Welded Pipe with Excellent Low Temperature Toughness

API X80 Grade Electric Resistance Welded Pipe with Excellent Low Temperature Toughness JFE TECHNICAL REPORT No. 18 (Mar. 2013) NAKATA Hiroshi *1 KAMI Chikara *2 MATSUO Nobuyuki *3 Abstract: This paper

### ALLOY 2205 DATA SHEET

ALLOY 2205 DATA SHEET UNS S32205, EN 1.4462 / UNS S31803 GENERAL PROPERTIES ////////////////////////////////////////////////////// //// 2205 (UNS designations S32205 / S31803) is a 22 % chromium, 3 % molybdenum,

### Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied

Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the

### Ch. 4: Imperfections in Solids Part 1. Dr. Feras Fraige

Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain

### Fatigue :Failure under fluctuating / cyclic stress

Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue

### The Clausius-Clapeyron Equation:

Chapter 10 Solid Solutions and Phase Equilibrium What is a phase? Phase Diagram Basics A phase diagram represents what phases are present at a given pressure, temperature and composition. Virtual maps

### Martensite in Steels

Materials Science & Metallurgy http://www.msm.cam.ac.uk/phase-trans/2002/martensite.html H. K. D. H. Bhadeshia Martensite in Steels The name martensite is after the German scientist Martens. It was used

### Concepts of Stress and Strain

CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original

### In order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 10-3 m. Thus,

5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,

### UR 317L: A 3%Mo minimum austenitic stainless steel (317L grade) Thermal conductivity (W m - 1 K - 1 ) Resistivity

Indu UR 317L UR 317L: A 3%Mo minimum austenitic stainless (317L grade) UR 317L (317L) is an austenitic stainless with a 3% molybdenum addition. Alloy UR 317L (317L) exhibits an austenitic microstructure,

### Defects Introduction. Bonding + Structure + Defects. Properties

Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of

### Chapter Outline Dislocations and Strengthening Mechanisms

Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip

### Heat Treatment of Aluminum Foundry Alloys. Fred Major Rio Tinto Alcan

Heat Treatment of Aluminum Foundry Alloys Fred Major Rio Tinto Alcan OUTLINE Basics of Heat Treatment (What is happening to the metal at each step). Atomic Structure of Aluminum Deformation Mechanisms

### Comparison of Impact Properties for Carbon and Low Alloy Steels

J. Mater. Sci. Technol., 2011, 27(10), 931-936. Comparison of Impact Properties for Carbon and Low Alloy Steels O.H. Ibrahim Metallurgy Dept., Nuclear Research Centre, Atomic Energy Authority, Egypt [Manuscript

### Dr. Alaa A. The Iraqi Journal For Mechanical And Material Engineering, Vol. 10,No. 1, 2010

Dr. Alaa A. The Iraqi Journal For Mechanical And Material Engineering, Vol. 10,No. 1, 2010 1.1 Metallurgy of gray cast iron: Most of industrial automobiles companies produced the brake rotor part from

### Phase. Gibbs Phase rule

Phase diagrams Phase A phase can be defined as a physically distinct and chemically homogeneous portion of a system that has a particular chemical composition and structure. Water in liquid or vapor state

### Question 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm

14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.

### WELDING AND COATING METALLURGY

WELDING AND COATING METALLURGY 1 INTRODUCTION 4 1.1 ROLE OF CARBON IN STEEL 4 1.2 WELDABILITY OF STEELS 5 2 CRYSTAL STRUCTURE 7 2.1 SOLUBILITY OF CARBON 8 3 IRON - IRON CARBIDE PHASE DIAGRAM 9 3.1 AUSTENITE

### Phase Equilibria & Phase Diagrams

Phase Equilibria & Phase Diagrams Week7 Material Sciences and Engineering MatE271 1 Motivation Phase diagram (Ch 9) Temperature Time Kinematics (Ch 10) New structure, concentration (mixing level) (at what

### INFLUENCE OF Cr, Mn AND Mo ON STRUCTURE AND PROPERTIES OF V MICROALLOYED MEDIUM CARBON FORGING STEELS

Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC: 669.15'26'74'28-194 INFLUENCE OF Cr, Mn AND Mo ON STRUCTURE AND PROPERTIES OF V MICROALLOYED MEDIUM CARBON FORGING STEELS Nenad

### Chapter Outline Dislocations and Strengthening Mechanisms

Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip

### Damasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems:

Damasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems: Sharp edges on chef knives. Nitrobe 77 is dishwasher safe without risk of corrosion or edge

### X15TN TM. A high hardness, corrosion and fatigue resistance martensitic grade CONTINUOUS INNOVATION RESEARCH SERVICE.

TM A high hardness, corrosion and fatigue resistance martensitic grade CONTINUOUS METALLURGICAL SPECIAL STEELS INNOVATION RESEARCH SERVICE DEVELOPMENT Enhancing your performance THE INDUSTRIAL ENVIRONMENT

### Precipitation of carbides in Cr Mo V cast steel after service and regenerative heat treatment

ARCHIVES of FOUNDRY ENGINEERING Published quarterly as the organ of the Foundry Commission of the Polish Academy of Sciences ISSN (1897-3310) Volume 9 Issue 1/2009 97-102 22/1 Precipitation of carbides

### North American Stainless

North American Stainless Long Products Stainless Steel Grade Sheet AISI 310S S31008 EN 1.4845 AISI 314 S31400 EN 1.4841 INTRODUCTION Types 310S SS and 314 SS are highly alloyed austenitic stainless steels

### 8. Technical Heat Treatment

8. Technical Heat Treatment 8. Technical Heat Treatment 95 6 cm 4 2 0-2 -4 C 400 C C -6-14 -12-10 -8-6 -4-2 0 2 cm 6 723 C temperature C 1750 750 250 When welding a workpiece, not only the weld itself,

### Chapter 8. Phase Diagrams

Phase Diagrams A phase in a material is a region that differ in its microstructure and or composition from another region Al Al 2 CuMg H 2 O(solid, ice) in H 2 O (liquid) 2 phases homogeneous in crystal

### Evaluation of the Susceptibility of Simulated Welds In HSLA-100 and HY-100 Steels to Hydrogen Induced Cracking

Evaluation of the Susceptibility of Simulated Welds In HSLA-100 and HY-100 Steels to Hydrogen Induced Cracking R. E. Ricker, M. R. Stoudt, and D. J. Pitchure Materials Performance Group Metallurgy Division

### University of Portland School of Engineering LABORATORY OUTLINE: TENSILE TESTING OF STEEL & ALUMINUM ALLOYS (ASTM E8)

TENSILE TESTING OF STEEL & ALUMINUM ALLOYS (ASTM E8) To carry out a standard tensile test on specimens of a hot rolled steel (AISI 1045), Type 2024- T351 aluminum, polymers (UHMW-PE, acrylic) and, from

### Chapter Outline. Diffusion - how do atoms move through solids?

Chapter Outline iffusion - how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steady-state diffusion (Fick s first law)

### AUSTENITIC STAINLESS DAMASCENE STEEL

AUSTENITIC STAINLESS DAMASCENE STEEL Damasteel s austenitic stainless Damascene Steel is a mix between types 304L and 316L stainless steels which are variations of the 18 percent chromium 8 percent nickel

### WJM Technologies excellence in material joining

Girish P. Kelkar, Ph.D. (562) 743-7576 girish@welding-consultant.com www.welding-consultant.com Weld Cracks An Engineer s Worst Nightmare There are a variety of physical defects such as undercut, insufficient

### x100 A o Percent cold work = %CW = A o A d Yield Stress Work Hardening Why? Cell Structures Pattern Formation

Work Hardening Dislocations interact with each other and assume configurations that restrict the movement of other dislocations. As the dislocation density increases there is an increase in the flow stress

### INFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES

CO-MAT-TECH 2005 TRNAVA, 20-21 October 2005 INFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES Jiří MALINA 1+2, Hana STANKOVÁ 1+2, Jaroslav DRNEK 3, Zbyšek NOVÝ 3, Bohuslav MAŠEK

### Chapter Outline. Defects Introduction (I)

Crystals are like people, it is the defects in them which tend to make them interesting! - Colin Humphreys. Defects in Solids Chapter Outline 0D, Point defects vacancies interstitials impurities, weight

### A Study of the Properties of a High Temperature Binary Nitinol Alloy Above and Below its Martensite to Austenite Transformation Temperature

A Study of the Properties of a High Temperature Binary Nitinol Alloy Above and Below its Martensite to Austenite Transformation Temperature Dennis W. Norwich, P.E. SAES Memry Corporation, Bethel, CT Abstract

### A Comparison of FC-0208 to a 0.3% Molybdenum Prealloyed Low-Alloy Powder with 0.8% Graphite

A Comparison of FC-0208 to a 0.3% Molybdenum Prealloyed Low-Alloy Powder with 0.8% Graphite Francis Hanejko Manager, Customer Applications Hoeganaes Corporation Cinnaminson, NJ 08077 Abstract Iron copper

### Continuous Cooling Transformation (CCT) Diagrams

Continuous Cooling Transformation (CCT) Diagrams R. Manna Assistant Professor Centre of Advanced Study Department of Metallurgical Engineering Institute of Technology, Banaras Hindu University Varanasi-221

### HIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT

IJMC14-244-2 HIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT Copyright 215 American Foundry Society Abstract Simon N. Lekakh Missouri University of Science and Technology,

### Material data sheet. EOS Aluminium AlSi10Mg_200C. Description

EOS Aluminium AlSi10Mg_200C All information in this data sheet refers to the alloy EOS Aluminium AlSi10Mg_200C. This alloy is formed when the powder EOS Aluminium AlSi10Mg is processes at a building platform

### North American Stainless

North American Stainless Long Products Stainless Steel Grade Sheet 2205 UNS S2205 EN 1.4462 2304 UNS S2304 EN 1.4362 INTRODUCTION Types 2205 and 2304 are duplex stainless steel grades with a microstructure,

### Chapter 5: Diffusion. 5.1 Steady-State Diffusion

: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process

### Lösungen Übung Verformung

Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress- strain diagram? 2. Name the four main

### North American Stainless

North American Stainless Flat Products Stainless Steel Sheet T409 INTRODUCTION NAS 409 is an 11% chromium, stabilized ferritic stainless steel. It is not as resistant to corrosion or high-temperature oxidation

### EFFECT OF COPPER ALLOY ADDITION METHOD ON THE DIMENSIONAL RESPONSE OF SINTERED FE-CU-C STEELS

EFFECT OF COPPER ALLOY ADDITION METHOD ON THE DIMENSIONAL RESPONSE OF SINTERED FE-CU-C STEELS Michael L. Marucci and Francis G. Hanejko Hoeganaes Corporation Cinnaminson, NJ 08077 - USA Abstract Fe-Cu-C

### GENERAL PROPERTIES //////////////////////////////////////////////////////

ALLOY 625 DATA SHEET //// Alloy 625 (UNS designation N06625) is a nickel-chromium-molybdenum alloy possessing excellent resistance to oxidation and corrosion over a broad range of corrosive conditions,

### THREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL. Hossam Halfa

THREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL Hossam Halfa Steel Technology Department, Central Metallurgical R&D Institute (CMRDI), Helwan, Egypt, hossamhalfa@cmrdi.sci.eg;

### 14:635:407:02 Homework III Solutions

14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.

### EFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL

EFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL Ladislav KANDER a, Miroslav GREGER b a MATERIÁLOVÝ A METALURGICKÝ VÝZKUM, s.r.o., Ostrava, Czech Republic,

### PRELIMINARY BROCHURE. Uddeholm Ramax HH

PRELIMINARY BROCHURE Uddeholm Ramax HH Uddeholm Ramax HH Uddeholm Ramax HH provides several benefits: The product offers uniform hardness in all dimensions combined with excellent indentation resistance.

### Full Density Properties of Low Alloy Steels

Full Density Properties of Low Alloy Steels Michael L. Marucci & Arthur J. Rawlings Hoeganaes Corporation, Cinnaminson, NJ Presented at PM 2 TEC2005 International Conference on Powder Metallurgy and Particulate

### Binary phase diagrams

inary phase diagrams inary phase diagrams and ibbs free energy curves inary solutions with unlimited solubility Relative proportion of phases (tie lines and the lever principle) Development of microstructure

### Ref. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield

MTE 585 Oxidation of Materials Part 1 Ref. Ch. 11 in Superalloys II Ch. 8 in Khanna Ch. 14 in Tien & Caulfield Introduction To illustrate the case of high temperature oxidation, we will use Ni-base superalloys.

### Hardness Testing. Objectives

Laboratory 2 Hardness Testing Objectives Students are required to understand the principles of hardness testing, i.e., Rockwell, Brinell and Vickers hardness tests. Students are able to explain variations

### Properties and Welding Procedure for Grade 91 Alloy Steel

International Journal of Engineering Research and Technology. ISSN 0974-3154 Volume 6, Number 6 (2013), pp. 767-772 International Research Publication House http://www.irphouse.com Properties and Welding

### Vanadium in Cold-rolled Sheet Steels

International Seminar 2005 on Application Technologies of Vanadium in Flat Rolled Steels - 34 - Vanadium in Cold-rolled Sheet Steels John Speer Colorado School of Mines Golden, CO. USA The presentation

### Technical Data BLUE SHEET. Martensitic. stainless steels. Types 410, 420, 425 Mod, and 440A GENERAL PROPERTIES APPLICATIONS PRODUCT FORM

Technical Data BLUE SHEET Allegheny Ludlum Corporation Pittsburgh, PA Martensitic Stainless Steels Types 410, 420, 425 Mod, and 440A GENERAL PROPERTIES Allegheny Ludlum Types 410, 420, 425 Modified, and

### Problems in Welding of High Strength Aluminium Alloys

Singapore Welding Society Newsletter, September 1999 Problems in Welding of High Strength Aluminium Alloys Wei Zhou Nanyang Technological University, Singapore E-mail: WZhou@Cantab.Net Pure aluminium has

### Material data sheet. EOS Aluminium AlSi10Mg. Description

EOS Aluminium AlSi10Mg EOS Aluminium AlSi10Mg is an aluminium alloy in fine powder form which has been specially optimised for processing on EOSINT M systems This document provides information and data

### Effect of Temperature and Aging Time on 2024 Aluminum Behavior

Proceedings of the XIth International Congress and Exposition June 2-5, 2008 Orlando, Florida USA 2008 Society for Experimental Mechanics Inc. Effect of Temperature and Aging Time on 2024 Aluminum Behavior

### Continuous Cooling Bainite Transformation Characteristics of a Low Carbon Microalloyed Steel under the Simulated Welding Thermal Cycle Process

Available online at SciVerse ScienceDirect J. Mater. Sci. Technol., 2013, 29(5), 446e450 Continuous Cooling Bainite Transformation Characteristics of a Low Carbon Microalloyed Steel under the Simulated

### Introduction to Metallography

Introduction to Metallography Metallography has been described as both a science and an art. Traditionally, metallography has been the study of the microscopic structure of metals and alloys using optical

Stainless steel grade chart ATLAS STEELS METAL DISTRIBUTION Chemical analysis (%) specified C Si Mn P S Cr Mo Ni Other Austenitic stainless steels 253MA S30815 0.05 1.1-2.0 0.8 0.040 0.030 20.0-22.0 10.0-12.0

### North American Stainless

North American Stainless Long Products Stainless Steel Grade Sheet AISI 316 UNS S31600 EN 1.4401 AISI 316L UNS S31630 EN 1.4404 INTRODUCTION NAS provides 316 and 316L SS, which are molybdenum-bearing austenitic

### North American Stainless

North American Stainless Long Products Stainless Steel Grade Sheet AISI 304 UNS S30400 EN 1.4301 AISI 304L UNS S30430 EN 1.4307 INTRODUCTION: Types 304 and 304L are the most versatile and widely used of

### Material data sheet. EOS NickelAlloy IN625. Description

EOS NickelAlloy IN625 EOS NickelAlloy IN625 is a heat and corrosion resistant nickel alloy powder which has been optimized especially for processing on EOSINT M systems. This document provides information